CONTACT MECHANICS BASED MECHANICAL CHARACTERIZATION OF PORTLAND CEMENT PASTE

A Dissertation by

CHRISTOPHER ANDREW JONES

Submitted to the Office of Graduate Studies of Texas A&M University

in partial fulfillment of the requirements for the degree of DOCTOR OF PHILOSOPHY

December 2011

Contact Mechanics Based Mechanical Characterization of Portland Cement Paste Copyright 2011 Christopher Andrew Jones

CONTACT MECHANICS BASED MECHANICAL CHARACTERIZATION OF PORTLAND CEMENT PASTE

A Dissertation by

CHRISTOPHER ANDREW JONES

Submitted to the Office of Graduate Studies of Texas A&M University

in partial fulfillment of the requirements for the degree of DOCTOR OF PHILOSOPHY

Approved by:

Chair of Committee, *Zachary C. Grasley *
Committee Members, Robert L. Lytton

Dan G. Zollinger Amine A. Benzerga Head of Department, John M. Niedzwecki

December 2011

ABSTRACT

Contact Mechanics Based Mechanical Characterization of Portland Cement Paste. (December 2011)

Christopher Andrew Jones, B.A., Southwestern University; B.S., M.S.; Texas A&M University

Chair of Advisory Committee: Dr. Zachary C. Grasley

Current research interest in multi-scale modeling of cement paste requires accurate characterization of the time-dependent mechanical properties of the material, particularly the C-S-H phase. Nanoindentation is evaluated as a tool for measuring both the instantaneous and the short-term viscoelastic properties of cement paste. Atomic force microscopy (AFM) based indentation is compared to conventional nanoindentaion in measuring mechanical properties of cement pastes. Time-dependent solutions are derived to characterize creep indentation tests performed on hardened cement paste and to extract the time-dependent properties. The effect of approximating C-S-H

viscoelastic properties with a time-independent Poisson’s ratio is discussed, and arguments for utilizing a time-independent Poisson’s ratio for short-term response are presented. In evaluating AFM as a mechanical characterization tool, various analytical and numerical modeling approaches are compared. The disparities between the

The measured elastic Young’s modulus values acquired by AFM indentation tests are compared to Young’s modulus values from nanoindentation measurements from cement paste. These results show that the calcium silicate hydrate (C-S-H) phase of hydrated portland cement has different properties on the nanometric scale than on the micron scale. Packing density of C-S-H particles is proposed as an explanation for the disparity in the measured results.

The AFM measured uniaxial viscoelastic compliance values are compared to similar values obtained with traditional nanoindentation for the same material. The comparison of these results shows that the calcium silicate hydrate (C-S-H) phase of portland cement has similar but distinct properties on the sub micron scale than on the micron scale. Additionally, the effect of moisture is evaluated by controlling the relative humidity (RH) of the testing environment between 40% and 100% plus, or wet. The viscoelastic compliance appears to be highest at 40% RH and the material appears to be less compliant at higher relative humidity levels. Possible mechanisms controlling the viscoelastic deformation are presented and evaluated in conjunction with the moisture related poromechanical effect.

DEDICATION

I dedicate this dissertation to my sweet wife Lauren. Without her support, particularly in these last weeks and months, I doubt if I could have completed this goal.

ACKNOWLEDGEMENTS

I would like to thank a number of individuals for their help with this work. First, I must thank Dr. Grasley for his continual encouragement, technical and personal

guidance, and for providing me many opportunities for success. Second, I would like to thank Tony Ohlhausen for his large role in facilitating the experimental portion of my research. Without my time at Sandia National Laboratories, made possible by Tony, there is simply no way that I would be finishing up right now. Additionally, I would like to thank my other committee members, Dr. Lytton, Dr. Zollinger, and Dr. Benzerga for serving me with excellent technical instruction in the classroom and for providing excellent technical feedback on my work. Also special thanks are owed to Dr. Muliana and to Dr. Gharaibeh for filling at the defense at the last moment. I appreciate each of you immensely.

I would also like to thank Sandia National Laboratories, The National Institute for Nano Engineering, and the National Science Foundation for providing facility, organizational, and monetary support for my work here at Texas A&M. Without these resources, I believe that I would not be where I am.

Finally, I thank my parents for the opportunity and encouragement to initially pursue higher education and my wife Lauren for supporting me in so many ways in this process.

NOMENCLATURE

*a* contact radius

*A* Hammaker’s constant

AFM atomic force microscopy

C-S-H calcium silicate hydrate

*Cov* covariance

δ the depth of penetration of the indenter

*E* elastic Young’s modulus

### ( )

*E t * viscoelastic Young’s modulus

0, , , ,1 2 3

*E E E E*

### β

viscoelastic fitting parameters*F* force applied to the indenter

φ half angle of the conical indenter

*G* elastic shear modulus

### ( )

*G t * viscoelastic shear modulus

γ surface energy
*h* surface separation
0
*h * rigid separation

### ( )

*H t*Heaviside function

*J*elastic compliance

### ( )

*J t*viscoelastic compliance

*k* cantilever stiffness

κ Poisson-Boltzman exponent

*K* elastic bulk modulus

### ( )

*K t * viscoelastic bulk modulus

*M* indentation modulus

ν Poisson’s ratio

### ( )

*t*

ν viscoelastic Poisson’s ratio

*P* probability

*s*

*p * surface pressure

0

*P * maximum Hertz pressure

*r* radial coordinate for axisymmetry

*R* tip radius
RH relative humidity
*t * time
*l*
*t * loading time
*h*

*t * load holding time

*u*

*t * unloading time

θ dimensionless parameter for evaluation

τ characteristic time

*u* surface displacement

*w/c * water to cement

0

TABLE OF CONTENTS Page ABSTRACT ... iii DEDICATION ... v ACKNOWLEDGEMENTS ... vi NOMENCLATURE ... vii TABLE OF CONTENTS ... x

LIST OF FIGURES ... xiii

LIST OF TABLES ... xvii

CHAPTER I INTRODUCTION AND PROBLEM STATEMENT ... 1

II OBJECTIVES ... 9

Objective 1: Develop experimental characterization techniques ... 10

Elastic characterization ... 10

Viscoelastic characterization ... 12

Objective 2: Describe and interpret the nanomechanical-behavior of cement paste ... 13

Interpret AFM and nanoindenter results ... 13

Compare results and draw conclusions regarding the nanometric structure ... 14 III THEORY ... 16 Classic analytical ... 17 Surface forces ... 18 Geometry ... 21 Numerical ... 22

Attard’s self-consistent method ... 23

Advantages of the self-consistent method ... 27

Applicability of the self-consistent method ... 31

Viscoelastic theory ... 38

Background theory ... 39

Application of the correspondence principle ... 39

*Approximating constant K or constant ν ... 41*

CHAPTER Page

IV EXPERIMENTAL ... 47

Materials ... 47

Nanoindentation ... 48

Atomic force microscopy ... 52

Relative humidity control ... 57

Experimental challenges ... 59

V RESULTS ... 62

Elastic ... 62

Viscoelastic ... 66

Nanoindentation ... 66

Atomic force microscopy ... 77

VI DISCUSSION AND INTERPRETATION ... 85

Discussion of elastic results and mechanisms ... 85

Particle packing densities ... 86

Interspersed crystalline phases ... 86

Interpretation of elastic properties ... 87

Discussion of viscoelastic results and mechanisms ... 89

Nanogranular densification ... 89

Layer sliding ... 90

Poroelastic relaxation ... 90

Dissolution of load bearing phases ... 91

Consideration of each mechanism ... 92

Interpretation of viscoelastic properties ... 95

VII CONCLUSIONS AND FUTURE RESEARCH ... 96

Research summary ... 96

Conclusions ... 98

Future work ... 100

Future experimental work ... 100

Future modeling work ... 102

REFERENCES ... 103

APPENDIX A: MATLAB CODE FOR THE IMPLEMENTATION OF ATTARD’S SELF CONSISTENT METHOD ... 118

APPENDIX B: NANOINDENTER TEST DATA ... 130

APPENDIX C: ATOMIC FORCE MICROSCOPE TEST DATA ... 136

Page VITA ... 170

LIST OF FIGURES

Page Figure 1: A conceptual force versus displacement curve for an arbitrary material

*where the slope, S, defines the stiffness or modulus of the material. ... 10
*
Figure 2: A schematic representation of the difference in probe size between

typical nanoindentation probes and AFM probes. ... 11 Figure 3: The colloidal model for C-S-H consists of multiple levels of

agglomerated particles that are held together by some sort of Van der

Waals type surface forces. ... 14 Figure 4: A) As two arbitrary bodies come into contact, separation dependent

surface forces (assumed to obey a Lennard-Jones form) dictate that there must be a region of repulsive action and an attractive region. The forces are a function of separation between the bodies which is in turn a function of radial position for curved bodies. B) In the case of indentation, the force applied to the indenter body deforms the

material being indented and the area of repulsive surface forces grows as the contact area increases while the attractive zone remains roughly

constant. ... 19 Figure 5: A realistic indentation probe could be considered conical or spherical

depending on the depth of the indentation. The potential assumed

geometries are shown by the dashed lines. ... 22 Figure 6: A flow chart representing the self-consistent method [90] shows the

equations and the routine for simulating an indentation experiment. ... 26 Figure 7: The idealized cono-spherical tip geometry representing a diamond cube

corner probe at *h =*_{0} 42nmgenerated with the self-consistent solution.
The inset shows that the surfaces never “touch” with realistic

separation dependent surface forces. ... 28 Figure 8: The simulated pressure profiles for an AFM probe with tip radius 2 nm

at several indentation depths show the ability of the self-consistent solution to capture both repulsive and adhesive effects. Also plotted are the Hertzian pressure profiles for the same indentation depths. Notice that because the Hertz solution neglects the adhesion outside the area of contact, the overall magnitude of the pressure profile is

Page Figure 9: AFM based indentation data for cement paste indented with a diamond

cube corner probe are fitted with the self-consistent, Hertz, and

Sneddon solutions. The data shown are obtained from the retraction of the probe from the hydrated cement surface to minimize incorporation of plasticity. The Hertz and self-consistent solutions are virtually

identical for *h <*_{0} 0. ... 33
Figure 10: Typical low force elastic indentation data obtained with a typical

AFM imaging probe with tip radius ≈3 nmfor very shallow

indentation depth indicates the ability of the self-consistent solution to
model the pre-contact behavior readily observed in AFM experiments.
The inset shows the typical contact (e.g. *h <*_{0} 0) regime that highlights

the difference between self-consistent and analytical models. ... 34 Figure 11: As θ decreases, the error introduced by using the analytical solutions

rapidly increases. Since some of the parameters that define θ are experimentally controllable, AFM based indentation experiments can be designed such that minimal error is introduced by modeling with

analytical solutions. ... 37 Figure 12: For a constant bulk modulus, common intermoduli relationships

dictate that if the shear modulus decreases with time, the viscoelastic

Poisson’s ratio must increase. ... 42 Figure 13: The nanoindenter used in this study was the Hysitron Triboindenter.

This device is a flexible, stand-alone nanomechanical testing system and is widely considered the industry standard for nanoindentation

testing. ... 49 Figure 14: A schematic representation of the loading for the creep

nanoindentation tests shows the rapid loading followed by a holding phase and finally the unloading of the material. The loading and unloading slopes are not realistic and are only intended to demonstrate

that the load is applied and removed over a finite period of time. ... 50 Figure 15: A schematic representation of an atomic force microscopy probe

shows the deflection of the cantilever being generated by the movement of the base of the cantilever. The deflection of the cantilever and the movement of the actuator define the penetration

Page Figure 16: The Dimension Icon system used in this research was actually

manufactured by Veeco before the acquisition of the AFM division of Veeco by Bruker. The instrument used in this research was identical

to the device pictured here except for the Bruker logo [114]. ... 54 Figure 17: The conceptual representation of the time-dependent indentation

experiment performed in this research illustrates that with step actuator movement the cantilever deflection is reduced due to material

relaxation. ... 56 Figure 18: The customized bubbler system for controlling the relative humidity

of the portland cement paste during AFM indentation tests works by

blending “wet” gas with dry gas to achieve a desired relative humidity. ... 59 Figure 19: The long term drift inherent to the atomic force microscope made long

term creep testing of the material difficult. ... 60 Figure 20: A) The elastic Young’s modulus measured with AFM shows an

apparent bimodal distribution while B) Young’s modulus measured

with nanoindentation [44] shows a multimodal trend. ... 63 Figure 21: A typical AFM topographical image of cement paste seems to support

the colloidal structure of C-S-H. Inscribed on the image are

representations of the approximate contact areas of the AFM probe and

a typical nanoindentation probe at maximum indentation depth. ... 65 Figure 22: Typical 30 s nanoindentation displacement versus time plot including

the fit function. The data has been time shifted so that *t t t*= − * _{l}*. ... 68

Figure 23: The fit function *h t plotted using the mean values of*

_{( )}

*E*

_{0},

*E , and*

_{1}β

calculated from the 30 s tests and from the 1 hr tests. ... 70 Figure 24: For conical indenters, as the penetration depth (displacement)

increases the contact area must increase, thus reducing the applied stress for a constant load. These curves assume a constant load of

and a typical Berkovich indenter. ... 71 Figure 25: Histograms for the fit parameters obtained from the 30 s creep

Page Figure 26: The probability density plots of (a) and (b) showing the trimodal trend

of measured displacements and viscoelastic properties extracted from the nanoindentation tests. Darker areas indicate higher probability, while dashed lines indicate mean values for each Gaussian probability

density function. ... 77 Figure 27: Typical creep indentation test data obtained with AFM showing the

best fit line obtained using (29). ... 78 Figure 28: The calculated fit parameters obtained from fitting the 30 second

experimental data with(29) at 40% RH, setting τ* _{i}* =0.3,3,and 30s. ... 80

Figure 29: The instantaneous response from the loading portion of the creep
indentation (or *E*_{0}from (37)) shows the stiffest instantaneous response

at 90% RH. ... 81 Figure 30: The normalized viscoelastic compliance measured on samples

exposed to different relative humidity values shows that the greatest relaxation occurs with the driest sample. The error bars on this plot

represent one standard deviation from the mean in each direction. ... 82 Figure 31: The normalized viscoelastic compliance measured with AFM and

nanoindentation at RH = 40% in each case. The error bars in this figure represent one standard deviation from the mean in each

direction. ... 83 Figure 32: The poromechanical effect is only relevant at high moisture levels and

the fact that greater relaxation was measured at low relative humidity levels suggests that other time dependent deformation mechanism(s)

LIST OF TABLES

Page Table 1. Fit parameters for the 30 s load holding data and for the 1 hr load

holding data. ... 69 Table 2. Fit parameters for the 30 s load holding data obtained at various relative

CHAPTER I

INTRODUCTION AND PROBLEM STATEMENT

Portland cement concrete is a heterogeneous composite composed of portland cement, water and natural mineral aggregates that is the most widely consumed

manmade material worldwide [1]. Despite being widely used for over a century, various problems still plague concrete infrastructure today such as chemical attack [2], limited freeze thaw durability [3], and reinforcement corrosion [4]. Furthermore, concrete structures tend to be difficult and expensive to retrofit or repair when unexpected problems do arise [5].

Despite the ubiquity of concrete, many of its fundamental material properties, particularly at small length scales, are not well understood. This is likely due to the lack of a regular microstructure in the portland cement paste. The calcium silicate hydrate (C-S-H) phase of the cement paste is generally understood to be crystalline on the atomic to molecular scale and amorphous on any larger scale [6]. The C-S-H phase is of particular interest since its properties tend to control the properties of the bulk concrete. Unfortunately, since the microstructure and fundamental deformation mechanisms are not very well understood, predicting mechanical properties from material inputs has not progressed much from the early empirical work of Abrams [7].

____________

With the recent interest in muli-scale constitutive modeling of infrastructure materials, the promise of accurate mechanical predictions from mathematical models has created some excitement in the materials community. For example, CEMHYD3D, created at the National Institute for Standards and Technology, provides realistic three dimensional microstructure and can be used with finite element modeling to predict elastic properties for cement paste [8]. Current efforts aim to create similar models for predicting viscoelastic properties.

Given the multi length scale heterogeneity of cement paste, fundamentally accurate models must account for mechanical behavior on these different length scales. In an effort to effectively model the multi-scale response of portland cement concrete, experimental techniques are required that characterize the material on ever shorter length scales. In addition to providing intrinsic input properties for multi-scale models [9-13] for predicting the macroscale behavior of cement paste and concrete, measuring

fundamental mechanical properties on the micro to nanometer length scale enhances the understanding of concrete deformation mechanisms. The indentation technique provides an excellent means for obtaining the mechanical properties from a localized region of a material.

Recent technology has made measurement of mechanical properties on these ever-decreasing length scales possible. The nanoindentation technique is particularly appealing for use on cement paste because the small probe dimensions allow

measurement of the properties on short enough length scales to discern heterogeneity in mechanical properties. Furthermore atomic force microscopy (AFM) provides an even

smaller probe that can be used to extract properties from yet shorter length scales [14-18]. Nanoindentation has long been the method of choice for micromechanical characterization of all sorts of materials [19-23], but when applied to cementitious materials, the interpretation of the measured results are complicated by the somewhat ambiguous nanostructure of the calcium silicate hydrate (C-S-H) phase of portland cement paste.

Several studies have been conducted using the nanoindentation technique on cement and concrete to measure elastic properties. Velez et. al performed

nanoindentation experiments on portland cement clinker and measured properties for the main phases [21]. Multiple studies have investigated the elastic properties of hydrated portland cement paste [24-30] with various experiments and calculations.

Nanoindentation has also been used to measure elastic properties of phases in atypical cements and cement composites [15, 23]. The existence of low density and high density C-S-H first proposed by Jennings and collaborators [31-33] was later utilized as an explanation for the bimodal distribution of elastic properties measured by Ulm and collaborators [34-36]. Trtik et al. [37] suggested that the presence of varying amounts of crystalline products (such as unhydrated cement or calcium hydroxide) within the

nanoindentation interaction volume provide a more likely explanation for the measured bimodal distribution of elastic properties when ostensibly indenting C-S-H. However, Ulm et al. [38] subsequently provided evidence that large enough compositionally homogenous regions exist in hardened cement paste such that the nanoindentation interaction volume may often be a (compositionally) single phase; as such, the bimodal

distribution of measured elastic properties in indentation of cement paste would suggest two types of C-S-H. More recent studies have proposed the existence of a third distinct phase or a trimodal distribution of measured elastic properties [29, 39].

The mechanical properties of hardened portland cement paste have been shown to be time dependent by various experimental methods, (e.g. [40-44]) and the time dependency has traditionally been attributed to the C-S-H phase of the paste. While the nanoindentation technique has most often been used for determination of elastic

properties, recently the technique has been applied to measure time-dependent mechanical properties as well. This time dependency has generally been considered detrimental; however, if this time dependent mechanical behavior of C-S-H were better understood, perhaps it could be used for beneficial purposes such as mitigating shrinkage cracking or facilitating healing of cementitious materials. In the present work, the term “viscoelastic” will be used in a very broad sense to encompass any sort of time

dependent mechanical behavior to include viscoplasticity, apparent viscoelasticity arising from poromechanical relaxation, and true viscoelasticity.

The specific mechanism responsible for the time dependency of the mechanical properties of portland cement paste is not clear from the literature and is likely not a single specific mechanism but rather a combination of different mechanisms acting in concert. Powers offered one of the earliest discussions of the phenomenon and

suggested that creep of concrete is related to the seepage of physically bound water into the capillary pores of the pasted thus creating an apparent viscoelastic effect [45]. Power’s theory is commonly referred to as seepage theory in the literature. Feldman

hypothesized that creep in cementitious materials is related to the formation of new interlayer space as the C-S-H crystallizes and this mechanism is referred to as the

interlayer theory in the literature [46]. The rearrangement of C-S-H particles in response to localized shear stress has been theorized as the mechanism responsible for creep of cementitious materials by several researchers [43, 47-49]. This mechanism of

viscoelastic response is known as the viscous shear theory, and is presented in different forms relating to the assumed structure of the C-S-H. Cementitious materials have also been considered poromechanical materials by various researchers [50-52]. The

poromechanical response is related to the movement of fluid within the porous cement paste in response to pressure gradients from the applied mechanical stress, but is distinct from the seepage theory in that it only considers unbound water that can readily flow through the pore network. As a result, the poromechanical response of cement paste is considered only a short term phenomenon. Additionally, a more recently proposed mechanism involves the dissolution and reformation of load bearing phases in response to stress applied to the paste [53].

While numerous studies have investigated the elastic properties of cement paste using nanoindentation, fewer studies have been conducted that investigate the

nanoindentation technique as a tool for measuring viscoelastic properties of cementitious materials. Vandamme and Ulm provide solutions for the problem of time-dependent indentation and perform some experiments to validate the solutions [54]. Additionally, Vandamme and Ulm show that the measured “creep modulus” indicates the presence of low density C-S-H, high density C-S-H, and an ultra-high density C-S-H [55]. Nemecek

et. al also considered nanoindentation creep as it affects the measured elastic properties of cement paste [56].

Some general solutions for time-dependent indentation also exist in the literature. Cheng offers a viscoelastic solution for a spherical indenter [57] and a flat punch

indenter [58], neither of which extend well to more common conical indenters. Cheng and Cheng also provide an excellent review of various phenomena present in indentation including indentation solutions for viscoelastic materials [59] for constant displacement rate indentation tests. Other studies have been aimed at accounting for the viscoelastic dissipation that occurs when performing elastic indentations [56, 60]. Fischer-Cripps [61] proposed a straightforward, phenomenological solution to characterize indentation creep, but the solution is empirical and thus not useful for understanding fundamental material behavior.

To date the application of time-dependent nanoindentation to cementitious materials has been limited. This study aims to characterize the short-term time-dependent viscoelastic Young’s modulus of C-S-H using nanoindentation. Various assumptions made while formulating a time-dependent indentation solution will also be analyzed and a generalized solution for time-dependent indentation response of a viscoelastic material to a step loading will be presented.

Nanoscale mechanical characterization of portland cement paste has yielded interesting new findings about this ubiquitous construction material but has also raised many questions as well. There exists a great deal of ongoing discussion regarding the

interepretation of nanoindentation results obtained from testing portland cement. Specifically in question is the source of the multimodal distribution of measured properties reported in virtually every nanoindentation based study of portland cement paste [25, 27, 29, 30, 34-36, 62-65]. Ulm et al. assert that the source of the distribution of measured mechanical properties could be attributed to distinct levels of packing density within the C-S-H. Lura et al. suggest that there may be other explanations for the distribution including the inclusion of ostensibly stiffer nano-crystalline phases present in the C-S-H phase, all within the interaction volume of an individual indentation test [37, 66]. Both explanations are tractable and have basis in well established existing theories. The packing density explanation owes to the colloidal model for C-S-H first proposed by Powers [67] and then later developed by Jennings and coworkers [33, 35, 41, 68-70]. Similarly, crystalline hydration products have long been known to exist in hydrated portland cement [53] and the mechanical properties of the crystalline phases do differ from those of the C-S-H phase [71]. Chen et al. confirmed existence of nano-crystalline phases present within C-S-H that could influence nanoindentation results [25]. It should be noted that neither explanation necessarily excludes the other and that the debate on this topic has mainly centered on determining the most likely explanation for the mostly undisputed experimental results.

Atomic force microscopy based indentation can illuminate this discussion to some degree because the AFM probe interacts with a smaller volume of material than is typical of nanoindentation experiments. A reduction in interaction volume should reduce the effect of the porosity, causing the measured values to approach those of the

intrinsic C-S-H particles. The measurement of mechanical properties with AFM is not a new idea, but obtaining consistent, accurately calibrated properties from AFM based indentation experiments has proved difficult. Furthermore, since nanoindentation produces perfectly acceptable results for homogeneous materials, the added complexity of AFM based measurements makes AFM based indentation less appealing for large classes of materials. Nevertheless, given the heterogeneous structure of C-S-H on the micron to nanometer scale, useful and distinct information can be gained from AFM that is not garnered from nanoindentation.

AFM based characterization of portland cement paste has been initiated by various researchers. Mondal et al. performed nanoindentation experiments coupled spatially with AFM to correlate various results with particular morphological phases [16]. Similarly, Saez de Ibarra et al. used AFM and nanoindentation to characterize cement paste with carbon nanotube dispersions [15]. More recently, Kim et al. used atomic force acoustic microscopy to measure the elastic properties of portland cement paste [72]. None of these approaches use the AFM probe as one would use a

nanoindenter to extract a force versus displacement curve to characterize the material elastic properties.

CHAPTER II OBJECTIVES

The primary objectives of this study are to experimentally measure the

instantaneous and time-dependent mechanical properties of portland cement paste with AFM on the sub-micron length scale and to differentiate these measured results from analogous results obtained from traditional nanoindentation on the micron length scale. This study will address the interpretation of AFM indentation data and provide insight into the application of various approaches for modeling AFM indentation.

To date the application of time-dependent nanoindentation to cementitious materials has been limited. This study aims to characterize the short-term time-dependent viscoelastic Young’s modulus of C-S-H using nanoindentation. Various assumptions made while formulating a time-dependent indentation solution will also be analyzed and a generalized solution for time-dependent indentation response of a viscoelastic material to a step loading will be presented.

Additionally, the elastic properties of C-S-H will be experimentally measured on the tens-of-nanometers length scale with AFM and these measurements will be used to help illuminate the discussion surrounding the multimodal distribution of C-S-H mechanical properties measured with nanoindentation. The proposed mechanisms of time-dependent deformation within C-S-H will be reviewed and hypotheses will be made to explain the difference in measured viscoelastic compliance obtained with nanoindentation and with AFM.

Objective 1: Develop experimental characterization techniques

Elastic characterization

The technique of choice for interrogation of material properties at the micro to
nano scale has been, and likely will continue to be, nanoindentation, although relatively
few researchers have applied this technique to cement paste or concrete [15, 34, 36,
73-75] and all have been relatively recent. Nanoindentation involves the instrumented
loading of a surface with a sharp probe while monitoring the applied force, *F*, and the
displacement into the surface, δ . For an arbitrary material a conceptual force versus
displacement curve can be found in Figure 1.

**Figure 1: A conceptual force versus displacement curve for an arbitrary material **
**where the slope, S, defines the stiffness or modulus of the material. **

Indentation
Depth
Fo
rc
e
Ap
pl
ied
*dForce*
*S*
*dDepth*
=

The probe is pushed into the material and is then retracted and the slope of the initial portion of the retraction curve is most closely tied to the elastic properties of the material since this response does not include plasticity.

For this study, portland cement paste will be indented with a traditional nanoindenter and with AFM to compare the indentation size effect. Though the same property is measured the results are not the same since the interaction volumes of the two different probes are quite a bit different. Figure 2 shows the relative difference in size for typical nanoindenter and AFM probe tips.

**Figure 2: A schematic representation of the difference in probe size between typical **
**nanoindentation probes and AFM probes. **

The Berkovich tip, which was used for traditional nanoindentation testing in this study, has a typical tip radius of 150 nanometers while a typical AFM imaging tip is on the

R=150nm

Berkovich _{Cube Corner} _{AFM Imaging Tip}

R=40nm

R=8nm

74˚ 49˚

16˚

order of eight nanometers. A cube corner tip which could potentially be used on either instrument has a typical tip radius of 40 nanometers. Furthermore, the tip angle should be considered. For the Berkovich tip with a typical half angle of 74°, the contact area and the interaction volume change very quickly with increased indentation depth. Conversely, tips with smaller half angles preserve a smaller indentation volume at deeper indentation depths compared to the Berkovich tip.

The elastic properties of C-S-H will be experimentally measured on the tens-of-nanometers length scale with AFM and these measurements will be used to help

illuminate the discussion surrounding the multi modal distribution of C-S-H mechanical properties measured with nanoindentation, which probes the hundreds to thousands of nanometers length scale.

Viscoelastic characterization

Though often treated strictly as an elastic material for design purposes, the mechanical properties of portland cement concrete are known to have a history effect or memory [42, 76, 77]. It is possible that a more complete understanding of the

fundamental nature of the time dependent deformation mechanisms in the C-S-H phase of the cement paste could lead to processing, mixture, design, or placement techniques that could optimize the performance of portland cement concrete.

Analogous to the perception of concrete as a time-independent material, the nanoindentation technique has most often been used for determination of elastic

mechanical properties as well. Viscoelastic nanoindentation testing involves the

instrumented loading of a surface with a sharp probe while monitoring the applied force
as a function of time,*F t*( ), and the displacement into the surface as a function of time,

( )*t*

δ . Viscoelastic experiments can be cast into general categories: creep tests

(controlled force), relaxation tests (controlled displacement), mixed creep and relaxation, and oscillatory.

With the traditional nanoindenter, the force applied to the probe is easily controlled and the creep test is the most practical. With AFM, neither force nor

displacement are totally controllable, and the analysis of the experiment becomes more complicated as it involves mixed creep and relaxation. In this study both traditional nanoindentation and AFM will be used to measure viscoelastic properties of the cement paste.

Objective 2: Describe and interpret the nanomechanical-behavior of cement paste

Interpret AFM and nanoindenter results

In general, the cement paste has higher elastic modulus and lower viscoelastic compliance when tested with AFM than with nanoindentation. This difference will be explained from a microstructural perspective, particularly the micro and nano porosity present in the C-S-H phase of the cement paste. The disparity in elastic results is somewhat obvious, but the difference in viscoelastic properties is less so. This study will address the interpretation of AFM indentation data and provide insight into the application of various approaches for modeling AFM indentation.

Compare results and draw conclusions regarding the nanometric structure

The reduced elastic modulus measured with nanoindentation versus AFM, coupled with the colloidal spheres model [31, 33, 41, 69, 70] for C-S-H microstructure implies that there may be two or more different packing densities of crystalline spheres within the H. In the context of coordination number, the individual spheres of C-S-H are more coordinated within the colloidal groups, than the colloidal groups are coordinated with one another. Figure 3 schematically shows the colloidal model for C-S-H in portland cement.

**Figure 3: The colloidal model for C-S-H consists of multiple levels of agglomerated **
**particles that are held together by some sort of Van der Waals type surface forces. **

*20 nm*
≈

The colloidal spheres model for C-S-H provides a convenient explanation for the distribution of mechanical properties observed with nanoindentation, but this

explanation should not be seen as causal. Other models exist for the structure of C-S-H such as the Feldman-Serada model [78, 79] and other theories exist to explain the modality observed in the results of nanoindentation testing [37, 66].

CHAPTER III THEORY

This chapter will develop the theory that will be used to model the experimental results presented in Chapter V. The chapter will begin with a general introduction to contact mechanics: the description of how bodies deform against one another. The specific issues that manifest with small length scale and small load contact will be analyzed and evaluated. Finally, time dependent solutions for describing viscoelastic contact will be formulated.

Utilization of either a nanoindenter or atomic force microscope to extract mechanical properties necessitates employment of contact mechanics. The contact problem was first solved by Hertz [80] as a means of calculating the deflection of optical lenses when stacked against one another and, as a result, the Hertz solution describes the elastic contact of spherical bodies. More recently, Galin and Sneddon provided a contact solution for a cone with an elastic half space [81, 82]. Since the AFM and

nanoindentation probes used in this study can be approximated as conical in shape, and are penetrated into the cement paste to a significant enough depth such that the sides of the probe dominate the contact area, the Galin-Sneddon solution provides a better starting point than the Hertz solution for this application. Indentation is also similar to the Boussinesq problem of a rigid foundation interacting with an elastic half space. The primary difference between the classic analytical contact theories is the geometry of the body interacting with the elastic half space. More recently, numerical approaches have

been proposed that avoid some of the simplifying assumptions present in each of the analytical theories.

Classic analytical

The two most common contact theories regularly in use are the Hertz and Sneddon theories and the major difference in these theories involves the assumed geometry of the contact, or for indentation, the assumed shape of the indenter being used to press into the material and the related pressure field in the contact area. In the case of Hertzian

*indentation, the indenter is a half sphere of radius R [80]. The central equation of the *
Hertz solution that relates indentation depth to load may be cast as

1/2 3/2

### 4

### 3

*F*

### =

*M R*

### δ

, (1)

*where F is the load applied to the spherical indenter, δ is the indentation depth, and M*
is the indentation modulus expressed as

2 2
1 1
1 *material* *indenter*
*material* *indenter*
*M* *E* *E*
ν ν
− −
= +
,
(2)

*where E is the elastic Young’s modulus, *

_{ν}

is the Poisson’s ratio, and the subscripts
denote whether the property is of the indenter or of the material being indented. For
*diamond indenters (E~1TPa), the second term in (2) is often negligible such that*

2 2
1 1
*material*
*material*
*E* *E*
*M*
ν ν
≈ =
− − _{.} (3)

In traditional nanoindentation and with many AFM probes, pyramidal indenters are the norm and can be idealized as conical. The Galin-Sneddon solution is appropriate for these experiments and the solution for conical indentation can be cast as

### ( )

2*2M Tan*

*F*

### φ

### δ

### π

= , (4)where φis the half angle of the conical indenter probe [81, 82]. Equations (1) and (4)

*can be used to fit experimental force versus displacement data and determine M for the *
indented material.

Surface forces

Classical contact mechanics has adequately described the interaction and

deformation between bodies in the cases of micro and nanoindentation for many years,
but with the increase in popularity of AFM, new questions have been raised regarding
the applicability of classical solutions to the AFM contact problem. Since the attractive
forces measured with AFM are approximately the same order of magnitude as those
applied to the AFM probe, ignoring adhesive surface forces may result in significant
error. Figure 4 schematically shows a generalized contact scenario and a generalized
indentation scenario. For two axi-symmetric bodies or for an axi-symmetric indenter
and a flat surface, the separation between the bodies *h* varies as a function of the radial
coordinate*r*. For most materials, the combination of varied surface separation as a
function of position and general surface physics causes the indenter probe to experience
both attractive and repulsive forces while in contact.

**A
** **B
**

**Figure 4: A) As two arbitrary bodies come into contact, separation dependent **
**surface forces (assumed to obey a Lennard-Jones form) dictate that there must be a **

**region of repulsive action and an attractive region. The forces are a function of **
**separation between the bodies which is in turn a function of radial position for **
**curved bodies. B) In the case of indentation, the force applied to the indenter body **
**deforms the material being indented and the area of repulsive surface forces grows **
**as the contact area increases while the attractive zone remains roughly constant. **

While separation dependent surface forces do exist in micro and nanoindentation experiments, generally the load applied to the indenter tip is so much larger than the contribution of the adhesive surface forces, that the surface forces can simply be

neglected. The bodies experience various surface forces which in aggregate can often be adequately described by the empirical Lennard-Jones potential function [83].

The Lennard-Jones model proposes that the two bodies in question experience negligible surface forces at large separations, attractive surface forces at intermediate

u Repulsive zone Attractive zone Attractive zone

separations, and repulsive surface forces at very small separations (what would generally be known as “in contact”). The Lennard Jones equation can be cast as

12 6
0 0
3
( )
6
*s*
*z* *z*
*A*
*p h*
*h* *h* *h*
π
⎡_{⎛} _{⎞} _{⎛} _{⎞} ⎤
= ⎢_{⎜} _{⎟} −_{⎜} _{⎟} ⎥
⎝ ⎠ ⎝ ⎠
⎢ ⎥
⎣ ⎦_{,}
(5)

where

*p h*

_{s}_{( )}

is the pressure profile between the two bodies as a function of surface
separation *h*

_{, }

*z is the equilibrium separation distance, and A is Hamaker’s Constant,*0

which can be related to the interfacial surface energy of the interacting bodies according
to
2
0
16
*A*
*z*
γ
π
= . (6)

For the purposes of this study, γ is not precisely the intrinsic interfacial surface energy of the interacting indenter and substrate; rather, it is a sum of surface energy, meniscus forces, and electro-chemical forces. The Lennard-Jones expression has the advantage of describing both the attractive and repulsive phenomena known to exist in contact

mechanics of most materials. For minimally adhesive materials, or for large indentation depths where the adhesive contribution to the total force is minimal compared to the repulsive contribution, a simpler Poisson-Boltzman repulsion form may be more appropriate [84]. The exponential repulsive form considered here is

### ( )

9 0*h*

*s*

*r*

*r*

*z*

*p h*

*P e*

*P*

*h*κ − ⎛ ⎞ = +

_{⎜}

_{⎟}⎝ ⎠ , (7)

where *P controls the magnitude of the pressure and κ and _{r}*

*z control the separation at*0

which the interaction takes place. The term *z is taken to be small so that the second *_{0}
term in (7) dominates the pressure response at small separations and prevents negative
values of *h*from being encountered in the simulation.

Two primary analytical theories exist that account for the influence of adhesive surface forces on the contact problem. The solution proposed by Johnson, Kendall, and Roberts (JKR) [85] accounts for adhesion within the area of contact while the solution proposed by Derjaguin, Muller, and Toporov (DMT) [86] considers adhesion outside the area of contact. Both the JKR and DMT theories account for the effect of adhesive surface forces but both do so while making assumptions about the region of contact and the pressure profile between the interacting bodies. Furthermore, both theories are applicable to spherical contact which does not generally extend well to conical indenters. Also, neither theory describes the interaction between bodies in the pre-contact regime.

Geometry

All of the analytical contact theories make assumptions regarding the geometry of the bodies that are in contact with one another. As mentioned previously, the Hertz theory assumes contact of spherical bodies while the Sneddon theory represented in (4) assumes the contact between a cone and a flat half space. In general, true indentation probes are neither simply conical nor spherical. Figure 5 schematically demonstrates how a realistic AFM or nanoindentation probe might look.

**Figure 5: A realistic indentation probe could be considered conical or spherical **
**depending on the depth of the indentation. The potential assumed geometries are **

**shown by the dashed lines. **

With respect to the assumption of a particular geometry, the researcher would need to know how deep the probe penetrates the material. In practice, this determination is fairly straight forward, particularly for the nanoindenter which presses very far into the material. However, for the AFM based indentation tests with very low applied forces, the indentation depth of the real probe may make this determination ambiguous.

Numerical

A few numerical solution approaches have been formulated for modeling contact problems. The solution proposed by Paul and Hashemi focused on accounting for non spherical geometries often encountered in real engineering problems and was solved by assuming positive pressure within the “contact area” and zero pressure outside [87, 88]. Another method proposed by Kalker involves minimizing elastic strain energy by

iterating pressure and deformation profiles and also assumes no interaction outside the contact area [89]. A more recent numerical solution method was proposed by Attard that makes fewer assumptions and is therefore considered to be potentially more accurate [90-94]. Attard’s method assumes that small deformation elasticity applies, and that all displacements occur in the vertical direction.

Attard’s self-consistent method

Attard’s self-consistent approach involves modeling the surface forces such that their affect on the indenter pressure profile is separation distance dependent [90, 91]. In other words, the axisymmetric pressure profile between the indenter and the material being investigated is

( ) *s*( ( ))

*s*

*p r* = *p h r* _{, } (8)

where *p is the surface force profile and _{s}*

*h r*

_{( )}

is the separation between the surfaces at a
radial coordinate*r*. Furthermore, the separation of the surfaces can be determined by subtracting the surface displacement

*u r*

_{( )}

from the separation expected if the motion
were considered rigid, such that
### ( )

0### ( )

### ( )

*h r* =*h r* −*u r* _{, } (9)

where *h r*_{0}

_{( )}

is the rigid separation (negative indicating interpenetration of the original
undeformed surfaces) for the two surfaces. The surface displacement may be expressed
as
### ( )

1*p h ss*

### (

### ( )

### )

*u r*

*M*

*r s*

*ds*π − = −

### ∫

, (10)*where dsis the element of the area over which the integration takes place, and s is *
simply a spatial variable in the plane that bisects the axis of contact.

The self-consistent approach conceptually mimics a displacement controlled indentation experiment. The method begins with the indenter and the material far apart such that no surface force is expected. In this initial state it is assumed that

### ( )

### ( )

0### ( )

0*u r*

*h r*

*h r*= =

_{.}(11)

Then, the indenter makes one small step toward the material such that the new

0*new* 0*old*

*h* =*h* + , where Δ is small (on the order of Δ 10−10to10−11meters). With a new *h , *0

a new displacement, *u r*

_{( )}

*, is guessed according to,*

### ( )

*0*

_{guess}### ( )

_{new}### ( )

_{old}*u r* =*h r* −*h r* . (12)

With the guessed displacement, a new separation,*h r*

_{( )}

, can be calculated with (9) and a
new pressure profile can be calculated with (8) and either (5) or (7). With a new
pressure profile, a new displacement, *u r*

_{( )}

*, can be calculated. This calculated*displacement profile is then blended with the guessed displacement from (12) at a prescribed mixing ratio to create a new “guessed” displacement profile and the loop is started a new. For each

*h step, this loop will continue until the difference between the*

_{0}newly calculated displacement profile and the previously guessed displacement profile

differ by a small amount,

### 1 10 m

−12### ×

in this case. Once the error in the deformation is minimized, a new*h step is made and the process is repeated for each*

_{0}

*h step. This*

_{0}process is illustrated in Figure 6 in flow chart form.

The self-consistent numerical method yields many advantages and some

disadvantages over analytical solutions. First,*h r*

_{( )}

, *u r*

_{( )}

, and*p h r*

_{(}

_{( )}

_{)}

are determined
(and recorded) at every step, in addition to simply recording the force. Recording these
quantities yields a wealth of information that is not available in the analytical solutions.
However, the major problem with this method is the computational expense required to
arrive at a solution. Since each incremental step must be iterated to find the correct
displacement and separation, the process can be computationally expensive.
Additionally, the value of Hamaker’s constant is generally not known a priori for most materials. Drawbacks aside, the Attard method of modeling the contact between two bodies is the most general approach currently in use.

**Figure 6: A flow chart representing the self-consistent method [90] shows the **
**equations and the routine for simulating an indentation experiment. **

( )
( ) 0( )
0
*u r*
*h r* *h r*
=
=
Probe
far
from
surface

### ( )

*guess*0

### ( )

*new*

### ( )

*old*

*u r* =*h r* −*h r*

Surface deflection guessed

h0step

Separation
and
pressure
calculated
( ) ( ) ( )
( ) ( ( ))
0
*s*
*guess*
*p r* *p h r*
*h r* *h r* *u* *r*
=
= −

New
deflection
calculated
( ) 1 *s*( ( ))
*calculated*
*p h s*
*u* *r*
*M* *r s* *ds*
π
−
=
−
∫
New
h0step
and
repeat

### (

### )

### (

2### )

0.5*n*

*ucalculated*

*uguess*

*Error*

*N*Σ − = Error calculated Is error < max error? Yes ( ) ( ) 0

*new*0

*old*

*h*

*r*=

*h*

*r*+ Δ

No *u r*

_{( )}

*i*=

_{guess}*f u*

### (

_{calc}_{( ) ( )}

*r u r*,

*−1*

_{guess}i### )

Make new guess from the calculationIs h0= h0 final? No End simulation Yes

Advantages of the self-consistent method

As alluded to above, the self-consistent method has two primary practical

advantages compared to traditional analytical techniques. First, given the generalization of the self-consistent method by Graham et al. [17], realistic tip geometries can be considered for any axi-symmetric indenter shape. Second, realistic surface forces and their related pressure profiles can be considered. Figure 7 shows a simulated indenter probe with a 40 nm tip radius and an included cone half angle of 48.5°, which represents a typical cube corner indentation probe.

The benefits of accurately accounting for the actual tip geometry in an indentation experiment depends on the particular experimental conditions, specifically, the

indentation depth compared to the characteristic geometry of a particular tip. For example, if a spherical indenter is displaced to a depth much less than the radius of the spherical tip, then the geometric assumptions of the Hertz solution are perfectly

acceptable [95, 96]. Similarly, if a cono-spherical tip is indented such that the depth of penetration is much greater than the radius of the conical tip, then the geometric

assumptions of the Sneddon solution are suitable [97]. The advantage of the self-consistent method is that the geometry of the contact is accounted for at any indentation depth.

**Figure 7: The idealized cono-spherical tip geometry representing a diamond cube **
**corner probe at ***h =*_{0} 42nm**generated with the self-consistent solution. The inset **
**shows that the surfaces never “touch” with realistic separation dependent surface **

**forces. **

With AFM based indentation, one approach has been to use relatively large spherical probes with low applied forces in an effort to meet the conditions of the Hertz solution [94]. This approach unfortunately neutralizes one of the great advantages of AFM, which is the extremely small tip dimensions available and the potential for measuring properties of adjacent dissimilar materials. By accurately accounting for the tip geometry of sharp AFM probes, one retains the ability to extract accurate material properties from very small areas of a material sample. For large classes of materials such as composites and naturally heterogeneous materials like portland cement paste, the

-60 -40 -20 0 20 40 0 20 40 60 80 100 Tip Profile Undeformed Surface u(r) Verti cal Posi tio n (nm ) Radial Position (nm) -46 -45.5 -45 -44.5 -44 -43.5 -43 -42.5 -42 2 3 4 5 6 7 8 Ve rt ic a l Po si tio n ( n m ) Radial Position (nm) Substrate Material Indenter

material properties can vary on short length scales of the same relative magnitude as the tip dimensions.

The second major advantage of the self-consistent approach is the flexibility in the pressure profile between the indenter and the material. For the Boussinseq problem to be analytically solved, a mathematical form of a pressure profile must be assumed. For example, in the case of the Hertz solution, the pressure is of the form of an ellipse such that,

### ( )

1/2 2 0 1 2*r*

*p r*

*P*

*a*⎛ ⎞ =

_{⎜}−

_{⎟}⎝ ⎠ , (13)

where *P is the maximum pressure and *_{0}

*a*

is the radius of the circular “contact area”.
The first major advantage of accurate geometric accounting is also related to the second
major advantage through the concept of contact area in the analytical expression of
### ( )

*p r* given in (13). As is expected from an understanding of realistic surface forces, the
two surfaces in contact never actually “touch.”1

1_{ In continuum mechanics, the idea of “contact” is ambiguous since bodies are assumed }
to be comprised of points having no dimension, but no two points are allowed to coexist
in the same space.

This separation between the two surfaces, even at positive applied force levels, is
preserved in the self-consistent solution and is shown in the inset in Figure 7. Since the
self-consistent method only predefines the pressure-separation relationship, this allows
for a more general *p h r*

_{(}

_{( )}

_{)}

and, as a result, a more general solution to the contact
problem.
Figure 8 shows the calculated pressure profiles at multiple indentation depths determined from a simulated experiment with a typical silicon AFM imaging probe and portland cement paste. It is interesting to note that as the indentation depth increases, the shape of the pressure profile changes to match the shape of the indenter, since the

repulsive contribution dominates the *p h r*

_{(}

_{( )}

_{)}

response. Also plotted in Figure 8 is (13)
plotted at the same indentation depths with *a*

assumed to equal the *r*position

corresponding to the inflection point of the numerically generated pressure profile. The
particular *P value chosen for the solid curves in Figure 8 were determined by matching *_{0}
the total force applied to the indenter probe. Since the Hertz solution does not account
for adhesive surface pressure clearly shown, the peak repulsive pressure in the Hertzian
case is lower than that generated by the self-consistent solution.

**Figure 8: The simulated pressure profiles for an AFM probe with tip radius 2 nm **
**at several indentation depths show the ability of the self-consistent solution to **
**capture both repulsive and adhesive effects. Also plotted are the Hertzian pressure **

**profiles for the same indentation depths. Notice that because the Hertz solution **
**neglects the adhesion outside the area of contact, the overall magnitude of the **

**pressure profile is reduced to achieve an equivalent total applied force. **

Applicability of the self-consistent method

Given the computational expense needed to implement the self consistent method, particularly when compared with the relative simplicity of analytical solutions, one naturally questions when the extra effort is necessary. This subsection aims to identify conditions where the self consistent method of modeling AFM contact provides tangible benefit over analytical solutions.

-1 -0.5 0 0.5 1 1.5 0 0.5 1 1.5 2 2.5 3 h 0=-0.75 h 0=-0.5 h 0=-0.25 h 0=0 Hertz -0.75 Hertz -0.5 Hertz -0.25 Hertz 0 Pre ssur e (G Pa ) Radial Position (nm) Centerline of axisymmetric indenter

As alluded to in the previous sections, the applicability of an analytical solution may depend on the particular experimental conditions, or conversely, the necessity of the more cumbersome self-consistent solution may depend on specific experimental

conditions. With this in mind, several AFM indentation tests are modeled with both
analytical solutions and the self-consistent method. First, Figure 9 shows a typical force
*( F ) vs h data from an AFM indentation test fitted with Hertz, Sneddon, and self-*_{0}
consistent models. These data were obtained with a diamond cube corner tip with an
effective tip radius of 40 nm. The loads applied to the tip in this case are in the range of

µN, which is roughly comparable to very low nanoindentation loads.

*Best fit values for the Hertz and Sneddon solutions for the fit parameter M were *
coincidentally both found to be 42 GPa while the self consistent solution yielded

45GPa. Figure 9 shows that for this experiment, the self-consistent model does not provide a substantially better description of the experiment than the analytical solutions.

**Figure 9: AFM based indentation data for cement paste indented with a diamond **
**cube corner probe are fitted with the self-consistent, Hertz, and Sneddon solutions. **

**The data shown are obtained from the retraction of the probe from the hydrated **
**cement surface to minimize incorporation of plasticity. The Hertz and **

**self-consistent solutions are virtually identical for ***h <*_{0} 0**. **

The results in Figure 9 should not be generalized, however, as the applicability of the self-consistent routine is highly dependent on the experimental conditions. Figure 10 shows a typical indentation test performed on cement paste with a very small probe and a very shallow indentation depth. For these data, the probe has a tip radius of

approximately 2 nm and the maximum force is in the tenths of nanonewtons. -10 0 10 20 30 40 50 60 -60 -40 -20 0 20 40 60 80 Measured Attard S/C Hertz Sneddon Force (µ N) h 0 (nm)

**Figure 10: Typical low force elastic indentation data obtained with a typical AFM **
**imaging probe with tip radius **≈3 nm**for very shallow indentation depth indicates **

**the ability of the self-consistent solution to model the pre-contact behavior readily **
**observed in AFM experiments. The inset shows the typical contact (e.g. ***h <*_{0} 0**) **
**regime that highlights the difference between self-consistent and analytical models. **

The most noticeable improvement that the self-consistent approach gains over
the analytical solutions is the description of the pre-contact behavior. The inset in Figure
10 highlights the traditional contact region (i.e. *h <*_{0} 0). Since the analytical contact
theories are only defined in the repulsive contact regime, the pre-repulsive (adhesive
force) region is not described in either the Hertz or the Sneddon theories. Furthermore
in terms of fitted elastic indentation modulus, there is great disagreement between the

### -0.4

### -0.2

### 0

### 0.2

### 0.4

### 0.6

### 0.8

### -5

### 0

### 5

### 10

### 15

Measured Attard S/C Hertz Sneddon### F

### or

### ce

### (

### nN

### )

### h

0### (nm)

-0.2 -0.1 0 0.1 0.2 0.3 0.4 0.5 0.6 -0.8 -0.6 -0.4 -0.2 0 0.2 Fo rc e (n N ) h 0 (nm)models. The self-consistent model data shown in Figure 10 was generated with

5 GPa

*M =* , while the Hertz and Sneddon solutions yielded *M =*0.95 GPaand

10 GPa

*M =* , respectively, as best fit modulus values. Since neither analytical solution
accounts for the relatively large affect of surface forces in this test, the error introduced
by modeling with the analytical solutions is significant.

Two cases have been shown where AFM obtained indentation data has been fitted with Attard’s self-consistent solution and with traditional analytical solutions. For the data shown in Figure 9, the benefit of using the self-consistent solution to model the experimental data is negligible, while for the data in Figure 10 the self-consistent method is all but required. This section will conclude with an analysis of the relative accuracy of the analytical solutions versus the self-consistent method. A simple dimensionless parameter, θ , by which various test conditions can be compared was proposed by Fuller and Tabor [98, 99] and will be modified very slightly here. This parameter can simply be thought of as the force required to displace a given indenter to some depth in the material compared to the maximum adhesive pull off force exerted between that indenter and the material being tested, such that,

*indentation peak*
*attraction peak*
*F*
*F*
θ −
−
= . (14)

Specifically, the terms in (14) can be substituted with (1) or (4) in the numerator, depending on the maximum indentation depth and the geometry of the tip used, while the denominator can be defined as

4

*attraction*

*where for this case, R is the radius of the spherical indenter tip or the radius of the tip of *
the conical-spherical indenter tip. Eq. (15) may be recognized as the adhesive pull off
force term defined in [86]. For Hertzian indentation where the geometry is spherical or
where the indentation is spherically dominated

3/2
max
1/2
3
*M*
*R*

### δ

### θ

### γ

= , (16)and for Sneddon indentation where the indentation geometry is conically dominated

### ( )

2 max 2*M Tan*

*R*δ φ θ π γ = . (17)

As a way of characterizing the error one might encounter from applying an analytical solution versus the self-consistent numerical solution, one may define,

% *fitted* *simulation* 100
*simulation*
*M* *M*
*Error*
*M*
−
= × . (18)

*Figure 11 represents the error in fitted M (determined via analytical solutions) *
compared to the same value from Attard’s self-consistent numerical solution (*M _{simulation}*).
The data points in this figure were created by generating combinations of

, * _{Max}*, ,and

*M*

### δ

*R*

### γ

_{that resulted in θ values that were spaced over a large range. Next, the }self-consistent solution method was used to simulate indentation experiments with these combinations of input parameters and the force versus displacement data were exported and fitted with the Hertz, JKR, and DMT solutions to determine

*M*using a nonlinear

_{fitted}optimization routine in Mathematica. Finally the error for a given θ was computed with (18).

**Figure 11: As θ decreases, the error introduced by using the analytical solutions **
**rapidly increases. Since some of the parameters that define θ are experimentally **

**controllable, AFM based indentation experiments can be designed such that **
**minimal error is introduced by modeling with analytical solutions. **

Figure 11 shows that for high values of θ , the error introduced by modeling indentation experiments with analytical solutions is minimal, while as θ decreases the error increases rapidly. This is an important fact to note because the maximum

indentation depth and the tip geometry can be selected when designing the experiment.

10 20 30 40 50 60 70 80 1 10 100 1000 104 Hertz JKR DMT % Error θ

It is also interesting to note that for these simulated indentation tests, neither the JKR nor the DMT theories produce tangible benefit compared to the Hertz theory, though for traditional contact mechanics applications such as determining the contact area between bodies, the JKR and DMT theories may provide more benefit. In general, for δ =0,

both the JKR and DMT theories over predict the adhesive force compared to the self-consistent simulation. For experimental conditions where θ must be small such as very shallow indentation depth or very low modulus-high surface energy materials, numerical modeling such as the Attard self-consistent method should be employed to achieve accurate results.

Viscoelastic theory

A common method for deriving solutions to boundary value problems involving viscoelastic materials involves the elastic-viscoelastic correspondence principle in which field variables and constitutive properties in an elastic solution are replaced by the corresponding Laplace (or Fourier) transformed viscoelastic analogs, solved in the transform domain, and then inverted back to the time domain. Unfortunately, the correspondence principle generally precludes problems that involve time-dependent transition from traction boundary conditions to displacement boundary conditions (or vice versa) on the boundary of the bodies involved. However, Lee and Radok [100, 101] showed that transforms could be applied and accurate solutions obtained so long as the contact area between an indenter and the material being indented was monotonically increasing with time. In other words, for indenters of increasing cross section with